(2) Electroreflectance of GaSb from 0.6 to 26 eV Abstract. Schottky barrier electroreflectance spectra are reported for GaSb from 0.6 to 26 eV. Accurate energies are determined for a number of critical points between the sp3 and Ga−3d valence bands and the conduction bands. The energy of XV7 is shown to lie at least 3 eV below ΓV8. This is below the value obtained from local pseudopotential calculations and the x-ray photoemission assignments, but follows a trend previously established by nonlocal pseudopotential calculations for Ge and GaAs. The Ga 3d-XC6 exciton binding energy is of the order of 100 meV. Keywords. Ames Laboratory, Schottky barrier, pseudopotential Disciplines. Condensed Matter Physics | Physics Comments. This article is from Physical Review B 14 (1976): 4450, doi:10.1103/PhysRevB.14.4450. Posted with permission.. This article is available at Iowa State University Digital Repository: http://lib.dr.iastate.edu/physastro_pubs/46.

(3) PHYSICAL REVIEW. 15 NOVEMBER 1976. 14, NUMBER 10. VOLUME. B. of GaSb from 0.6 to 26 ev. Electroreflectance. D. E. Aspnes Bell Laboratories,. Murray Hill,. ¹wJersey 07974. C. G. Olson and D. W. Lynch Ames Laboratory,. Energy Research and Development. and Department. Administration. of Physics, Iowa State. University,. 50010 (Received 16 March 1976) Ames, Iowa. Schottky barrier electroreflectance spectra are reported for GaSb from 0.6 to 26 eV. Accurate energies are determined for a number of critical points between the sp' and Ga-3d valence bands and the conduction . This is below the value obtained from local bands. The energy of X7 is shown to lie at least 3 eV below calculations and the x-ray photoemission assignments, but follows a trend previously pseudopotential established by nonlocal pseudopotential calculations for Ge and GaAs. The Ga 3d-X, exciton binding energy is of the order of 100 meV.. I,. I. INTRODUCTION GaSb is an interesting material with respect to solid-state spectroscopy and energy-band theory. The lack of inversion symmetry leads to a much richer optical spectrum than for its closest groupIV counterpart Ge. Because the spin-orbit splitting of Sb is large, the critical-point structures tend to be spread out so that the major singularities are observed with less overlap than with other members of the III-V family. It is therefore possible to obtain a number of critical-point energ ies to high accuracy. GaSb should consequently provide an excellent test of recently developed nonlocal pseudopotential methods, ' ' which have calculated very successfully the energy bands of Ge and GaAs over a wide range of photon energies. Of particular interest. will be the capability of these techniques to deal with exchange, correlation, and relativistic effects which are substantially more important in GaSb than in other materials to which they have been applied. The primary purpose of this work is to obtain accurate energies for interband critical points in GaSb. Critical points measured include not only those from the sP' valence bands, but also from the Ga 3d core levels located approximately 19 eV below the top of the sp' valence bands. The Schottky barrier electroreflectance (ER) method" was used. Its sensitivity enabled us to resolve some new critical-point features. The identification of several of these cannot be made with the presently available information, which emphasizes further the need for an accurate energy-band calculation. The outline of the paper is as follows: Experimental details are summarized in Sec. II. Results are discussed in Sec. III according to major 14. critical-point groupings, with the critical-point energies summarized in Table I and the spin-orbit splittings in Table II. In Sec. IV, we compare briefly our results with the probable best' of several' currently available band-structure calculations for GaSb. Spin-orbit splittings are also We discuss compared to theoretical calculations. the interesting question of the energies of the X, and X, points. By comparing our core-level measurements with x-ray photoemission (XPS) measurements" locating Ga 3d and pressure measurements" locating X „we obtain a binding energy of 90 meV for the Ga 3d -X, exciton.. ". ". II. EXPERIMENTAL. reported here were obtained All measurements polished I 1llj p(Sb) suron a bromine-methanol face on an n-type single crystal of GaSb of carrier To remove any concentration ND= 1.1&&10" cm. '.. possibility of residual damage, the surface was anodized to form an 0.3-p, m oxide layer, which A 40-A film of Ni was was then stripped in HCl. evaporated as described elsewhere'" to form a Schottky barrier on this surface. To reduce oxidation effects in the Ni film, the sample was stored under vacuum prior to measurement in the vacuum uv except for one evaluation spectrum measured from 1.8-5. 5 eV just after evaporation. The evaluation spectrum was the same as later spectra taken under the same conditions, showing that oxidation effects were negligible. Measurements in the 0.6-6.2-eV spectral range were performed using standard quartz-optic techniques with equipment already described. ' A I'bS cell, a Si photodetector, and an EMI 9556QB photomultiplier were used for the spectral ranges 0.6-1.2, 1.2 —1.8, and 1.7-6.2 eV, respectively.. ". 4450.

(4) ELECTROREFLECTANCE OF GaSb FROM 0. 6 TO 26 eV. 14. The sample temperature for these measurements was of the order of 10 K (liquid He cold finger). The flux was nominally unpolarized. The monochromator was calibrated with a Hg spectral line. source. Measurements in the 5. 5-27-eV spectral range were performed using the high-energy photon source of the Synchrotron Radiation Center of the Physical Sciences Laboratory of the University of Wisconsin. All measurements were performed at a sample temperature of approximately 110 K (liquid N, cold finger), using techniques and apparatus that also have been described previousPredominantly p-polarized flux was rely. '" flected at a 60' angle of incidence to maximize" the signal-to-noise ratio in this spectral region. All spectra were measured using 103-Hz squarewave modulation from a typical value of +0.3 V in the forward direction to various reverse voltages up to the breakdown limit at -1.8 V. The maximum attainable surface field 5, at breakdown was calculated from ND=1. 1x10" cm ' a, nd" fp 15.7 to be 230 kV/cm. To check independently this value, 5, was also calculated from the Franz-Keldysch oscillations observed at maximum modulation for the Ep transition, using the asymptotic theory" to evaluate kQ from the energies at which the oscillations were tangent to their envelope. Using the heavy-hole reduced mass p~ =0.041m„" whose contribution to Schottky barrier ER dominates that of the light hole unless separated explicitly, we calculate 8, =230 kV/cm. This value, in excellent agreement with that calculated from the barrier potential and ND, confirms the value of ND in the barrier region and justifies the use of the barrier equation to calculate the surface field for other. ". '". "'". tion), are shown in Fig. 1. Energies of 0.822 0.005 and 1.575+ 0.005 eV were determined for the E, and E, +bp critical points, respectively, and are indicated by lines in the figure. These energies were obtained by fitting to the experimental curve over a limited energy range containing the structure a theoretical low-field two-dimensional. +. Mp. critical-point. =Re[Ce' (E E~+-fI') ']+6, where C, 0, E~, and I' are adjustable parameters and the baseline b is chosen to account for zero offset (if any). The curve-fit energy for E, was corrected by adding the exciton rydberg of 2 meV as calculated from the parameters of this material, The fitting procedure is an extension of the three-point method" that is better suited to digital computation and provides better averaging by using more of the line shape. The spin-orbit splitting calculated from these data is ~p =753+ 5 meV. These results are in essential agreement with previous absorption" and stress-modulated magnetoreflectance" data on P-type samples. The most reliable values of the E, critical-point energy and the spin-orbit splitting ~p are 0.8102 eV, and 749 meV, respectively. Our larger values can be understood as arising from degeneracy effects. Indeed, assuming an ideal parabolic band structure with m,* = 0.042m„" and N~ = 1.1 x 10" cm ', we calculate E~ -E~ =19 meV. Our observed difference of 12 meV for E, is less, possibly for a number of reasons including carrier freezeout and exchange effects which depress the interband energy separation with increasing impurity concentration. The discrepancy between spin-orbit splittings is less than 12 meV since it concerns. ". ". ". 50 GO. SHOWN. x10. 0 O. Eo+ h 0. 50—. ER spectra for the E, and E, +4p transitions, taken with h, = 90 kV cm ' (+0.30-0.00-V modula-. I. i. I. i. i. 10. AND DISCUSSION. A. Ep, Fp + Dp transitions. S b —10K. Cs=eokv cm '. i. III. RESULTS. ". ". ". uniformity.. ER function". ~/E. modulation levels. Since the determination of the critical-point energies was the main objective of this work, we have not analyzed line shapes in detail. Due to the relatively large doping, it was not possible to achieve simultaneously the low-field limit and the uniform-field condition for the Ep structure for any value of surface field. The E, transition clearly exhibited a line-shape evolution" toward the uni-. form-field limit with increasing reverse bias, as expected in the Schottky barrier configuration. Modulation conditions for spectra for criticalpoint energy analysis purposes were chosen to favor the l. ow-field condition at the expense of field. 445l. i. I. I. I. I. 1.5. E(ev). 1.. Schottky barrier ER spectrum of the Ep and @p+ +p transitions of GaSb. The location of the anomalous + p + +p structure is indicated by the dashed line.. FIG..

(5) D. E. ASPNES, C. G. OLSON, AND D. W. LYNCH. 4452. only the difference. in energy between the spinorbit split I,"", valence band and the heavy-hole 1, valence band. As in Qe, it appears that the lighthole 1", band does not contribute substantially to the total E, structure, as expected from densityof-states considerations. Two line-shape peculiarities in these structures are worth mentioning: the significant difference between the Eo and E, +60 line shapes, and the appearance of an anomalous structure (weak in Fig. 1) about 60 meV above E, +a, . This structure is strongly dependent on the value of the voltage for the positive half of the modulation cycle. The main E, +~, structure has the general appearance of aM, critical point, with small asymmetry corrections" from the optical properties of the Ni overlayer, field inhomogeneity effects, and electron-hole correlation effects. Since the transition type and the optical properties of GaSb and Ni at the E, threshold are nominally the same, the substantially different line shape for E, is at first sight surprising. The difference is probably due to the essential singularity of the light- and heavyhole valence bands for Eo, and more accurate linefor these singularities may shape calculations" resolve this problem. The anomalous structure in Eo+Qo is weak for modulation from +0.30 V, but it dominates the line shape for modulation from 0.00 V. It is seen at no other critical point in GaSb. We believe that it is related to a similar effect seen in InSb and InAs by Bottka et al. , which has been interpreted tentatively in terms of band-population effects.. I. ". ". ". ". ". "". B. E&, E& + 6& transitions. The E, and E, +~, line shapes shown in Fig. 2 are quite similar to those obtained in Schottky barrier ER measurements on other semiconductors. We find by curve fitting the critical-point energies 2. 195+0.010 and 2.625+0.010 eV for the E, and E, + 6 c ritical points, respectively. The spin-orbit splitting is 6, =430+ 10 meV. Stress measurements"'" place these transitions along A or I. , in agreement with similar materials; a line-shape analysis of heterojunction ER spectra" shows that M, critical points are responsible for the structures. The A, value is about 15jo less than that predicted. '". y. ". due to the influence by the simple two-thirds rule, of neighboring bands. Our energy values show some differences with respect to wavelength modulation results, which place the critical-point energies 30-90 meV lower as a result of the greater uncertainty in interpreting the features of the less-well-structured first-derivative line shapes. Spin-orbitsplitting values of 445, 442, and 438 meV,. ". "'". " ". ". &. I. &. 14. /. I. I. I. Ga Sb-10K ~s = 90kV cm. 40—. a.. I. I. (. 20—. CL. c3. O. 0. Et+. E) I. I. I. I. 2.0. I. I. I. I. 2.5. 3.0. E(ev) FIG. 2. Schottky barrier ER spectrum of the E, + 6& transitions of GaSb.. E& and. calculated from the first-derivative results, are closer to our value of 430+10 meV. The better agreement for b, , is not surprising since interpretational ambiguities are reduced for difference calculations. C. Eo triplet. The earliest interpretation of the weak Eo triplet structures as originating at"'" I' was later questioned in GaSb in favor of a 6 assignment. But symmetry analysis"'" of the Eo features in Ge identified the critical-point symmetry as I', and this was confirmed later by accurate critical-point energy measurements which showed for both Ge, ' and GaAs, ' an energy separation of the second and third structures equal to the spin-orbit splitting of. "'". the top of the valence band. Our values for the three E', critical-point energies are 3.191~ 0.005, 3.404+ 0.010, and 4. 160 +0.010 eV. These were obtained by curve fitting to line shapes taken with g, = 90 kV cm ', which are shown in Fig. 3. The energy obtained for the. highest-energy member is in principle less accurately determined due to its overlap with the X and E, structures, but this uncertainty was minimized by calculating a second derivative of the ER line shape (see Fig. 5 and associated discussion). The calculated spin-orbit splittings are 6,' =213 + 10 meV a.nd 60 =756+ 15 meV. The spin-orbit splittings are in good agreement with the values 216+ 5 and 745+ 5 meV obtained in metal-oxide-semiconductor (MOS) measurements on similar n-type GaSb by Parsons and Piller, although their critical-point energies are 30-40 meV low due to their (incorrect) assignment of the. ".

(6) ELECTROREFLECTANCE OF GaSb FROM 0. 6 TO 26 e& 4. '. I. I. I. I. !. I. I. I. I. ). I. I. 1. I. I. GoS. I. I. I. I. 1. GQsb-ioK. Cs-. 90 ky. cfTl-1. Eo+ho I. Eo. 4. I. I. I. I. I. I. I. I. 3.5. 5-0. E. l. I. I. I. 4.0. Ep{2) !. E~ {'I ). (eV). I. I. I. "'"'". fluenced by changes in lifetime broadening, which acts to spread the structures differently. The near degeneracy of I. and 6 critical points observed for.Eo in' GaAs appears to be missing in GaSb, although the line shape for Eo+ho indicates that some extra critical-point structure may be present. But this is not surprising since both I', and. I. ~8. are essential degeneracies.. As with QaAs, ' highly structured Schottky barrier EH spectra are obtained for GaSb in the vicinity of the F. peak. A typical spectrum obtained at h, =90 kVcm ' is shown in Fig. 4. In order to better resolve weak transitions appearing only as shoulders of stronger transitions, a higher-field ER syectrum (g, =240 kV cm ') was differentiated numerically twice with respect to energy. The result is shown in Fig. b. We consider first the dominant spectral features seen in Fig. 4. The E,'+6,'+~," structure at 4. 160 eV has already been discussed. The large feature near 4.40 eV labeled E,(1),E,(2) is a common feature of these materials. But for GaSb, it appears to be split into two components separated by an energy diffexence of the order of 30-40 meV, obtained by inspection of the anomalous width of the lower-energy half of the line shape. This splitting is too small to be ascribed to the spin-orbit interaction, and probably is a result of two critical points lying very close in both energy and wave vector. Further evidence for proximity follows from the decrease in apparent splitting with in-. ,. I. E fey). of GaSb.. critical-point energy to the positive peak on the ER spectrum. The observation of the valenceband spin-orbit splitting value near 6, = 749 meV for 6," confirms the assignment of I' symmetry for GaSb. We believe that our spin-orbit-splitting energies are more reliable than those of Parsons and Piller because their values were obtained from peaks alone, and consequently are in-. I. 5.0. FIG. 3. Schottky barrier ER spectrum of the Eo triplet. FIG. 4. Schottky barrier ER spectrum of the E2 complex of GaSh.. creasing field. ' Detailed energy-band calculations Ge locate the critical point(s) giving rise to '). A similar the E, structure in Ge near (~, 4, —, location is probable for GaSb. The peak in reflectance occux"s at 4. 35 eV, slightly lower in energy than E,. The location and symmetry of the third large transition, E, (3) at 4. 72+ 0.05 eV in Fig. 4, is not known. Several weaker structures are evident in the numerically differentiated spectrum of Fig. 5. Similar transitions near E, in GaAs were identified by polarization measurements on a {110jsurface and by the observation of a doublet-doublet energy sepRx'Rtlon Rs ox'lginRtlng from cl itlcal points neRr X.' No obvious doublet-doublet pattern is expected here because the calculated spin-orbit splitting of the valence band, g, =X, -X, , is 0.24 eV, about the same as that expected for the antisymmetric. for'. ". ". I. I. I. [. 2(. ). OJ. I. I. I. GaSb- )OK ~S = 240 kV cm '. I. 2 04 LLj. U. 0 lX. -2 C4. U. F +. ~o+~o X. {2) I. 45 E( eV). FIG. 5. Second energy derivative of a higher-field ER spectrum of the E2 complex of GaSb..

(7) D.. 4454. F. ASPNES, C. G. OLSON,. ". potential splitting of X, and X, . The X transitions should therefore spread over a range of the order of & eV. Since all four X transitions should possess reasonable and nearly equal oscillator strengths, it is clear from Figs. 3-5 that the lowest X transition . ) must lie at least as high as 4. 16 eV, the energy of Ep+4g+4p since there is no evidence of any critical-point structure below this or above Ep +4p. a range of over 0.5 eV. For if X7 X were to lie at or near E', +b, p at 3.5 eV, then at least one of the remaining X transitions should appear in the 3. 55-4.05-eV range. This is not observed. Due to the presence of the E, transitions, there is no obvious way to assign structures in the viFor want of a cinity of E, to the X quadruplet. better choice, we assign the 4.26-eV structure in . Although a number of possibilFig. 5 to X, ities exist for the remaining assignments, none are particularly satisfactory because of unacceptable variations in apparent oscillator strength or unrealistic energy separations. A further discussion of the energies of the critical points at X, with regard to core-level ER and x-ray photoemission (KPS) data" is given in Sec. IV.. g, -X,. -X,. D. E& complex. By contrast to GaAs, ' the E y complex lies in the quartz-optics range. Typical spectra, taken at a surface field of 90 kV cm ', are shown in Fig. 6. The dominant features here include the main peak with critical-point energy at 5. 59+ 0.03 eV, and the higher-energy component at 6.04+ 0.03 eV. The energy separation of 450+30 meV is in good agreement with the spin-orbit splitting, b, , =430. AND D. W. LYNCH. 14. z 10 meV, of the valence bands at A. This agreement, which is also nearly exact in a-Sn, ~ has been used to support a A - or L -symmetry origin for these critical points. But band-structure calculations" for GaP and GaAs, and the observation of a substantial difference between these spin-orbit splittings for Ge, and other semiconductors, has indicated that these critical points, if indeed near A, are off the symmetry axis for many of these materials. This may not be the case for. "". ". ". Gasb. Several weak structures also occur in the 5. 15.6-eV range. The two structures at o. 3V and 5.46 eV are remarkable for their sharpness. It is possible to correlate the 5.46-eV structure and the dip at 5.9 eV with transitions to the I. band since both are about 130 meV below the nominally E', and E y + Q I trans itions and their strengths are in proportion to the main structures. Therefore 130 meV becomes the spin-orbit splitting between L, , and I.~6, which is in good agreement with theory. But it is not clear why the oscillator strengths should be so weak for the transitions terminating. ... ". on the. I.4, band. E. Eo'. range. KR spectra in the vacuum uv spectral region from 6 to 12 eV are shown in Fig. 7. The highestenergy component of the E', complex in Fig. 6 appears at the far left and indicates the relative magnitude of the remaining structures. These spectra are considerably weaker than similar data for GaAs and" GaP owing to the difficulty of obtaining high surface fields in GaSb, a consequence of its relatively small band gap. The only unambiguous structure in this range is Eo' (I', —I', g with a critical-point energy of V. 9 *0.1 eV, which can be identified by its line-shape. ). E1+ 61. 0 CI. I. E). I. +6). LL. 0 Go Sb -10K. Cs=eokV cm '. 0. O Ga Sb. I. I. 5.5. 60O. l. 6.0. 10. E(eV). FIG. 6. Schottky barrier ER spectrum of the plex of GaSb.. —110K. 8, = 240 kV crn-~. E,. E E&'. com-. 12. (eV). FIG. 7. Schottky barrier ER spectrum of the 6-12-eV region of GaSb..

(8) ELECTROREFLECTANCE OF GaSb FROM 0. 6 TO 26 eV. 4455. similarity to the corresponding structure in GaP, at 9.38+ 0.1 eV in that material. Thus the conduction-band d-like bonding levels lie substantially lower in GaSb. The spin-orbit-split structure expected from I'~7 is absent, probably because of the small density of states from the small spin-orbitsplit hole mass. The remaining structures in this energy range are relatively broad, and probably occur in regions of low symmetry. No structures were observed in the energy range from 12 eV to the onset of core-level txansitions near 20 eV. This was due to the facts that the structure is broad even under the best of conditions, and that the fields obtained even at maximum possible modulation were relatively low.. F.. Core-level transitions. EH spectra for transitions between the Ga 3d core levels and the sp' conduction band are shown in Figs. 8 and 9. These data were obtained with a spectral resolution of 150 meV. Figure 9 shows in expanded form the critical-point structures between the spin-orbit-split j =-,' and ==, core levels,. X,. j. relative minimum. No evidence is seen for a critic31-point structure between the core levels and the I'~6 conduction-band absolute minimum, but this is expected from matrix element considerations. '0 In general, the core-level spectra of QaSb are more highly structured than those of QaP and GaAs, with more overlap between structures. This is not surprising in view of the downshift of the energies of all features of the sp' valence-conduction-band critical-point spectrum, which places more local conduction-band extrema within the exand the. conduction-band. GQSb -110K G~=240kvcm '. -60. FIG. 9. Schottky barrier ER spectrum of the Ga 3d -X& conduction-band critical points.. perimentally attainable energy range. A detailed analysis of the Ga 34~-XC transitions places the respective critical points at 19.82+ 0.05 and 20. 2'7+ 0.05 eV, giving a spin-orbit splitting az, =0.45+ 0.05 eV which agrees with that previously obtained for QaAs and GaP, 0 and also for QaSe. ' The strong feature that appears 1.8 eV above X, in both GaAs and GaP should be present near 21.6 eV in Fig. 8, but it seems to be extremely weak or absent altogether. Some evidence for the strong feature 3.0 eV above X, in GaAs and QaP is seen at 22. V eV, or 2.9 eV above X, in GaSb. The region of the conduction band giving rise to the latter transition therefore will bear an energy relationship to X, that is essentially independent of the potential of the anion. IV. DISCUSSION. E. (ev). FIG. 8. Schottky barrier ER spectrum of transitions from the Ga 3d core valence bands in GaSb.. The Schottky barrier ER spectra presented here contain a number of critical-point structures not previously observed. Some of these can be assigned, but others will require polarization measurements and more accurate band-structure calculations for their identification. To assist these calculations, more accurate critical-point energies are obtained for all higher-interband transitions for which positive identification can be made. The band-structure calculation of Cahn and Cohen, ' probably the best currently available for GaSb, predicts a number of critical-point energies that are given in Table I. The most serious discrepancies occur over 4 eV. As Cahn and Cohen point out' they were unable to remedy these discrepancies without causing unacceptable modifications of the lower-energy band structure within the local pseudopotential approximation, showing.

(9) D. E. ASPNES, C. G. OLSON, AND D. %. LYNCH. 4456. TABLE I. Energies of selected high-symmetry critical points of GaSb. The experimental values are determined fxom Schottky barrier EH data unless otherwise referenced. The theoretical values are fxom a local pseudopotential band-structure calculation by Cahn and Cohen. (Bef. 8). Exper iment. Transition. I C) (rY, &~. (~6. &~+~i. (I v Eo+&o. L. g. 0.8102 eV. -r,c). 2.43. C. ). 4.36 + 0.03. E2{2) (a, 4, 4) (~). 4.40 +0.03. E2(3) (~). 4. 72 + 0.05. (X, SY-&4Y,). D$. (from. transitions). 4c}. ~" t() =-'. -(~ =-')l ). Theoretical.. 756+ 15 213+ 10 430+ 10 450~ 30 ('P) 130 {~) 450+ 50. 260. 140 240 460. Beference 13. Reference 34.. 4. 160+ 0.02. (i, 4, z) (~). a,. Zg. Experimental.. 749 meV. triplet). Y 6o @6Y -X7). 3.404+ 0.010. I. - r,'). 6) (X ~~-I. 3.191~ 0.005. (r Y —rc8). (r'Y8. &o (from Eo ~o «8 — I'6). 2.625+ 0.010. -r,'). t+~s+glt (IV E2(1). ao. 0.9 eV. 2. 195+0.010. ~c). Y. Spin-orbit spl itting. Theory. 1.559. c). TABLE II. Spin-orbit splittings at selected high-symmetry critical points of GaSb. The experimental values are determined from Schottky barrier ER data unless otherwise referenced. The theoretical values are from Wepfer, Collins, and Euwema (Ref. 13), calculated using the Kohn-Sham-Gaspar exchange.. =171+ 15 meV). ' This suggests that it is almost. that the calculated spin-orbit splitting of the Ga 3d core state agrees almost exactly with experiment. Our lower limit of 4.25y0. 1 eV for the X", critical point can be used with the pressure deterrnination of the separation, 0.315 + 0.015 eV, to place an upper limit on the energy of X, . We note first that, although the pressure measurements were performed at room temperature and relevant ER measurements performed near liquid He temperature, the observed rigidity of the valence bands with temperature" together with the near equality of the temperature coefficients of" the Eo and" E, structures insures that no essential difference occurs in the I'ci-Xc splitting as the temperature is changed. Thus we find X, must lie at least (4.25+ 0.1 eV) —(0.810 eV) —(0.32 eV) =3.1+ 0. 1 eV below I'av. Structure assigned to X", (average of X, and X, ) has been observed in XPS measurements" at -2.7 eV. Using the calculated spin-orbit splitting, &, =0.24 eV, we find that the XPS value of the energy of X, relative to I', is -2.6 eV. Thus our "best" value for X, lies 0. 5 eV deeper than that obtained from XPS data, which in turn agrees with local pseudopotential predictions for most III-V materials where calculations are available. But we believe that our value should be in better agreement with the results of nonlocal pseudoyotential calculations, since one of the effects of the nonlocal yseudopotential is to spread the total width of the valence band. Specifically for Ge [the only material for which published data for X, (or Xv) are available], the nonlocal pseudopotential increases the Xv4-I v separation from 2.4 to 3.2 eV. ' By analogy, one may anticipate a lowering of X", , which should bring it into good agreement with the. entirely due to the spin-orbit splitting of the cation.. ER results.. x, -x,. It is interesting. 4.25 +0.1 4.61 ~0.05. (~). 4.74. -X,. + 0.05. ". 5.10 +0.03 5.20 +0.05. 5.37 1. (~e -&4.5) (~y ~C) (~ 4, 5-& 4, 5}. ~ C). Elk. Ic. (IY. (Ga 3dy — X6) (Ga 3d, g, -X, ) 2. (I. c6. X6 ) (indirect). + 0.03. 5.46 +0.02 5.59 + 0.03. 5.90 + 0.07 6.04 + 0.03. 6.9 7.9 19.82. + O. l. + 0.1 + 0.05. 20.27 + 0, 05. 0.43 + 0.2. 0.48. Reference 8. Reference 33. c From Hef. 33 with 4o value fx'om Heine gt ak. , Bef. 34.. that it is not adequate for the description of GaSb. Much better agreement is obtained with the spinorbit-splitting calculations of Wepfer et al. This is not surprising since the spin-orbit splittings depend more heavily on the atomic core potentials and are less influenced by crystal-field effects. Nevertheless, there are some discrepancies, notably in 4, and in b, The splitting 40 213+ 10 meV is remarkably small, being close to the value found in Ge (b. ' =200+ 3 meV)6 and in GaAs (b.. ". ,. ,. ". I', -X,.

(10) ELECTROREFLECTANCE OF GaSb FROM 0. 6 TO 26 eV. 14. 4457. Finally, we estimate the exciton binding energy between the Ga 3d valence band and the X, relative minimum of the conduction band. XPS results locate Ga 3d" at" -19.00~0. 15 eV relative to I", . Assuming the same relative shift between I', and 3d, ~, as measured for GaP, we convert this value to low temperature by adding 0.02 eV. The =~ level lies —, (0.45 eV) =0. 18 eV above this. Our measured Ga 3d, ~, separation of 19.82 eV therefore locates the X, singularity (the core level n =1 exciton line in the case of a sizeable interaction) at 1.02+ 0.25 eV. The X, energy can also be calculated by adding the E, gap at 110 K, 0.80 splitting, 0.31 eV. We find eV, to the I', X, =1.11 eV. The difference, 90+250 meV, is. the exciton binding energy of the core level. This is of the order of that previously measured for GaP and GaAs. '. ~J. C. Phillips and K. C. Pandey, Phys. Rev. Lett. 30,. Phys. 47 602 (1976). M. Haas and B. W. Henvis, J. Phys. Chem. Solids 23, 1099 (1962) . 3D. E. Aspnes, Phys. Rev. B 15, 4228 (1974). 24D. E. Aspnes, Phys. Rev. Lett. 31, 230 (1973). 5P. Lawaetz, Phys. Rev. B 4, 3460 (1971). D. E. Aspnes, Phys. Rev. B 12, 2297 (1975). D. E. Aspnes, Surf. Sci. 37, 418 (1973). D. E. Aspnes and A. Frova, Solid State Commun. 7, 155 (1969). 29 D. E. Aspnes and E. Rowe, Solid State Commun. 8, 1145 (1970); Phys. Rev. B 5, 4022 (1972). E. Rowe, Phys. Rev. Lett. 27, 188 D. E. Aspnes and (197 1) . E. Johnson and H. Y. Fan, Phys. Rev. 139, A1991. ". j. -X,. ". -X,. ". 787 (1973). K. C. Pandey and C. Phillips, Phys. Rev. B 9, 1552 (1974) . 3J. R. Chelikowsky and M. L. Cohen, Phys. Rev. Lett. 31, 1582 (1973) R. Chelikowsky and M. L. Cohen, Phys. Rev. Lett. 32, 674 (1974). W. D. Grobman and D. E. Eastman, Phys. Rev. Lett. 33, 1034 (1974); W. D. Grobman, D. E. Eastman, and L. Freeouf, Phys. Rev. B 12, 4405 (1975). D. E. Aspnes, Phys. Rev. Lett. 28, 913 (1972). D. E. Aspnes and A. A. Studna, Phys. Rev. B 7, 4605. J.. .. J.. J.. (1973). and M. L. Cohen, Phys. Rev. B 1, 2569 (1970). M. L. Cohen and T. K. Bergstresser, Phys. Rev. 141, 789 (1966). F. Herman, R. L. Kortum, C. D. Kuglin, and J. P. Van Dyke, in Methods in Computational Physics, edited by B. Alder, S. Fernback, and M. Rotenberg (Academic, New York, 1968), Vol. 8, p. 193. 'C. W. Higginbotham, F. H. Pollak, and M. Cardona, in Proceedings of the Ninth International Conference on the Physics of Semiconductors (Nauka, Leningrad,. R. C. Cahn. 1968), p. 57.. H. I. Zhang and J. Callaway, Phys. Rev. 181, 1163 (1969) ' G. G. Wepfer, T. C. Collins, and R. N. Euwema, Phys. Rev. B 4, 1296 (1971). '4L. Ley, R. A. Pollak, F. R. McFeely, S. P. Kowalczyk, and D. A. Shirley, Phys. Rev. B 9, 600 (1974). B. B. Kosicki, A. Jayaraman, and W. Paul, Phys. Rev. 172, 764 (1968) . D. L. Rode, B. Schwartz, and J. V. DiLorenzo, SolidState Electron. 17, 1119 (1974). ' A. A. Studna, Rev. Sci. Instrum. 46, 735 (1975). ' C. G. Olson, M. Piacentini, and D. W. Lynch, Phys. Rev. Lett. 33, 644 (1974). ' C. G. Olson and D. W. Lynch, Phys. Rev. B 9, 3159 (1974) . D. E. Aspnes, C. G. Olson, and D. W. Lynch, Phys. Rev. B 12, 2527 (1975). D. E. Aspnes, C. G. Olson, and D. W. Lynch, J. Appl.. .. ACKNOWLEDGMENTS. One of us (D. E.A. ) wishes to acknowledge useful discussions with E. O. Kane. We also express our appreciation to A. A. Studna and A. Pisarchik for their assistance in preparing the samples used in We have also benefitted these measurements. from the cooperation of E. M. Rowe and the Synchrotron Radiation Center Staff. The Synchrotron Radiation Center was supported by the NSF under grant No. DMR-74-15089.. J. J.. J.. (1965). M. Reine, R. L. Aggarwal, and B. Lax, Phys. Rev. B 5, 3033 (1972) . M. Reine, Ph. D. thesis (Massachusetts Institute of Technology, 1970) (unpublished), cited in Ref. 32. 34M. Reine, R. L. Aggarwal, and B. Lax, Solid State Commun. 8, 35 (1970). D. Sell, S. E. Stokowski,. R. Dingle, and J. V. DiLorenzo, Phys. Rev. B 7, 4568 (1973). D. E. Aspnes, J. Opt. Soc. Am. 63, 1380 (1973). 'J. E. Rowe and D. E. Aspnes, Phys. Rev. Lett. 25, 162 (1970). R. Enderlein, in Proceedings of the Twelfth International Conferenceon the Physics of Semiconductors, edited by M. Pilkuhn (Teubner, Stuttgart, 1974), p. 161. ~9R. Enderlein, P. Renner, and M. Scheele, Phys. Status Solidi B 71, 503 (1975). N. Bottka, R. Glosser, and J. Kinoshita, Bul. l. Am. Phys. Soc. 20, 287 (1975). 4 R. Glosser and B. O. Seraphin, Phys. Rev. 187, 1021 35D.. (1969). R. Glosser, J. E. Fischer, and B. O. Seraphin, Phys. Rev. B 1, 1607 (1970). 43N. Bottka and D. L. Johnson, Phys. Rev. B 11, 2969 44. (1975).. T. Tuomi, M. Cardona,. and. F. H.. Pollak, Phys. Status. Solidi 40, 227 (1970).. A. Ilier, E. Kierzek-Pecold, and Z. Werfel, Acta Phys. Pol. A 43, 55 (1973)..

(11) D. E. ASPNES, C. G. OLSON, AND D. %. LYNCH 46C. Alibert and G. Bordure, Phys. Status Solidi 40, 68v (19vo). 47L. M. Roth and B. Lax, Phys. Rev. Lett. 3, 217 (1959). 48R. R. L. Zucca and Y. R. Shen. , Phys. Rev. B 1, 2668. (1970).. J.. (19vo). 5~J.. P. Walter. and M.. L. Cohen, Phys. Rev. 183, 763. (1969).. and R. Braunstein, Phys. Rev. B 5, 497 (19V2). '"OM. Cardona, K. Shaklee, and F. H. Pollak, Phys. Rev. 154, 696 (1967). ~~J. C. PhiBips, in. Solid State I'hysics, edited hy F. Seitz and D. Turnbull (Academic, New York, 1966), Vol. 18,. 4~M. Welkowsky. p. 55.. J. E. Fischer, J. Matsuzaki, and W. E. Spicer, Phys. Rev. B 3, 4292 (1971). ~3D. D. Sell and E. 0. Kane, Phys. Rev. B 5, 417 (1972). 548. J. Parsons and H. Piller, Solid State Commun. 9, ~2T. M. Donovan,. v6v (19v1.). ~5J. A. Van Vechten,. ~6F. H. Pollak, M. Cardona, C. W. Higginbotham, F. Herman, and P. Van Dyke, Phys. Rev. 8 2, 352. Phys. Rev. 187, 1007 (1969).. L. Nosenzo, E. Reguzzoni, and G. Samoggia, Phys. Rev. B 9, 640 (1974). K. C. Pandey and J. C. Phillips, Phys. Rev. B 9, 1560. 58G. Guizzetti,. (19V 4).. P. Thiry, R. Pincheaux, D. Dagneaux,. and. Y. Petroff,. in Prooeedings of the Twelfth International Conferenc~ m the Physics of Semiconductors, edited by M. Pilkuhn (Teubner, Stuttgart, 1974), p. 1275. D. Auvergne, O'. Camassel, H. Mathieu, and M. Cardona, Phys. Rev. B 9, 5168 (1974). 6~D. E. Aspnes C. 6, Olson, and D. W, Lynch, Phys. Hev. B 14, 2534 (1976)..

(12)